Inorg. Chem. 1990, 29, 4059-4062 reducing agent other than CO, e.g. Zn, which can also serve as a chloride acceptor. If structure 2a is correct for the adsorbed tricarbonyl on SiOz and N a y , then there should be no reaction between the adsorbed carbonyl chloride and C O a t room temperature, since there is nothing that can serve as a chloride acceptor. This is indeed the case; no reaction is observed between 2a and C O (25 O C , 1 atm) after 24 h. Similarly, a reaction is to be expected between 2b on MgO and C O at room temperature. Although a reaction does occur, it is unfortunately not nearly as clean as previously observed on A1203. Thus, when 2b on MgO is treated with CO, a very complicated infrared spectrum is obtained. Some of the bands may be due to [ H R ~ ~ ( C 0 ) ~ , ] - ( a dbut s ) ,if this anion is present, it is not the major product. That a reaction takes place a t all however is consistent with MgO acting as a chloride acceptor. Conclusion Although R u ( C O ) ~ C I ~ ( T H Fis) spontaneously adsorbed by a
number of oxides, it is impossible to determine the surface structure of the adsorbed species simply by the infrared spectrum. Thus, a previous study on silica assigned the surface structure as Ru"(CO),(ads), a structure that does not contain coordinated chloride. It is apparent from the present study that a better description of the surface carbonyl on Si02and N a Y zeolite is Ru(CO),Cl,(ads). Only on the more basic oxides, Al2O3 and MgO, is chloride lost to yield the surface species R ~ ~ I ( C 0 ) ~ ( a d s ) . It is further proposed that the surface ligands include two oxides, 0-AI, so that the adsorbed tricarbonyl is not a formally cationic complex. Importantly, the distinction between the two surface structures is not readily made simply from the infrared spectra. The basic chemical reactions of the adsorbed carbonyls are required to confirm the proposed structures. Acknowledgment. Support for this work was provided by the National Science Foundation (Grant D M R 85-18364). B.E.H. acknowledges an A. von Humboldt fellowship during part of this work.
Contribution from the Department of Chemistry, Cornell University, Ithaca, New York 14853
Synthesis, Structure, and Properties of a New Ternary Metal Nitride, Ca3CrN3 Deborah A. Vennos, Michael E. Badding, and F. J. DiSalvo* Received February 27, 1990 We have synthesized a new ternary nitride, Ca,CrN,, from the binary nitrides at high temperature. The refined structure was solved in the Cmcm space group, Z = 4, with lattice constants (A) a = 8.503 (2), b = 10.284 (2), and c = 5.032 ( I ) and with R = 3.9% and R, = 3.9%. This new structure type consists of sheets of [CrN3I6 planar triangular units and calcium ions. Ca3CrN3 is insulating and paramagnetic with Cr3+in the low-spin state. This is the first unambiguous example of low-spin Cr3+. Larger than expected antiferromagnetic interactions produce a maximum in the magnetic susceptibility at 240 K, even though the shortest Cr-Cr distance is 4.73 A.
Introduction Although the chemistry of binary nitrides has been explored in detail, comparatively little work on ternary and quaternary nitrides has been reported. Preliminary work has shown that, in addition to the facile formation and stability of ternary nitrides containing electropositive elements, these phases exhibit a variety of novel properties. Examples include the N i d9 configuration in CaNiN,] the layered structures of MTaN? (M = alkali metal), and the unique structure types found in CazlFe3N17,3 Li3AINz,4 and CaGaN.5 These few examples suggest that ternary nitrides will display an extensive assortment of new compounds and structure types. We therefore undertook a large-scale investigation of alkaline-earth-metal- and transition-metal-containing nitrides. Herein, we report a new compound and structure type, Ca,CrN,, discovered initially as an impurity phase in reactions of Ca3N2 in stainless steel containers. Experimental Section Starting Materials. Chromium nitride was prepared by heating Cr powder (-100 mesh, 3N) in flowing nitrogen (prepurified by passing through finely divided copper at 150 "C and then activated alumina) at 800 "C for 1 day. The product was ground and reheated several times, yielding a mixture of CrN and Cr,N (approximately 50:SO). Granules of calcium (2N) were reacted at 1000 OC for 3 days in flowing nitrogen
The compound was then prepared as a majority phase by heating 0.2048 g of the CrN/Cr,N mixture (1.11 mmol of the hypothetical Cr,N2) and 0.601 1 g of Ca3N, (4.06 mmol) in a sealed stainless steel tube under an argon atmosphere at 1350 OC for 4 days, followed by cooling to 1050 "C in 5 h and finally cooling to room temperature in 12 h. There was no evidence of Ca3Nzremaining in the product mixture;
however, the brittle nature of the once malleable tube indicated that the excess Ca3Nzwas consumed by a reaction with the stainless steel. The product contained air-sensitive, burgundy needle crystals up to 1 mm in length, which were used for the structure determination. X-ray powder diffraction indicated a nearly pure Ca3CrN3 powder with a small unidentified impurity phase. The intensity of the strongest impurity diffraction peak was 6% as intense as the strongest peak of the majority
The material used for susceptibility measurements was prepared by heating a pressed pellet of an intimate mixture of 0.3103 g of CrN/Cr2N (1.69 mmol of Cr3N,) and 0.5070 g of CapNz(3.43 mmol) powders in a sealed molybdenum crucible under argon at the heating schedule mentioned above. The only impurity observable in the product by powder X-ray diffraction was Cr metal. The most intense Cr peak was only 6%
Chern, M. Y.; DiSalvo. F. J. Submitted for publication in J . Solid Sfate Chem. Jacobs, H.; von Pinkowski, E. J . Less-Common M e t . 1989, 146, 147. Verdier, P.; Marchand, R.; Lang, J . Rev. Chim. Miner. 1976, 13, 214. Juza, V. R.;Hund, F. 2. Anorg. Allg. Chem. 1948, 257, 13. Verdier, P.; L'Haridon, P.; Maunaye. M.; Marchand, R. Acfa Crysmllogr. 1914, 30, 226. I
(prepurified as above) to yield pure Ca3Nz. The binary products were identified by X-ray powder diffraction methods. Since both Ca3N2and Ca,CrN3 are air sensitive, all manipulations were carried out in an argon-filled glovebox. Synthesis of Ca3CrN,. The title compound was first discovered as a minority crystalline phase in a reaction of Ca3Nzand tin in a stainless steel tube. The bulk phase consisted of a gray powder, Ca3SnN,6with a minority phase consisting of needle crystals distributed throughout. Microprobe analysis of the crystals indicated the presence of calcium and chromium (a component in the stainless steel) at a Ca:Cr molar ratio of
( 6 ) Chern, M. Y . ; Vennos, D. A.; DiSalvo, F. J . To be published. 1
0 1990 American Chemical Society
Vennos et al.
4060 Inorganic Chemistry, Val. 29, No. 20, 1990
w' ' I '~ ' ' 1 Table 11. '
Positional Parameters for Ca,CrN, atom site X Y Ca 4c 0 0.1079 12) Ca 8g 0.2843 (2) -0.1174 ( i j 0.1945 (2) Cr 4c 0.5 N 4c 0.5 0.3757 (8) 0.1286 (6) 0.6918 (8) N 8g
0.25 0.25 0.25 0.25 0.25
Figure 1. Temperature dependence of the magnetic susceptibility of Ca3CrN1. Table 1. Summary of Crystal and Diffraction Data for Ca,CrN, space group Cmem (No. 63)
a. b, e.
cryst dimens. mm 20 m ,a?. deg; scan type octants measd X-ray radiation monochromator no. of measd reflcns no. of obsd reflcns' no. of independent reflcns abs coeff AL, mm-' R,b Rw: %
4 8.503 (2). 10.284 (2). 5.032 ( I ) 440 0.113 x 0.04 x 0.13 55; w-20 &h,k.l
Mo Ka graphite 577 303 263 5.79 3.9, 3.9
as intense as the strongest Ca3CrN3peak. Since the lower symmetry of Ca3CrN3splits the X-ray lines into many components, the impurity level of Cr was estimated to be less than 3 wt %. A larger percentage of Cr from the reaction mixture should have remained in the product; most of it must have alloyed with the molybdenum crucible, as it is not observed in the product. Magnetic Susceptibility. The magnetic susceptibility of the sample was measured by the Faraday technique in a previously calibrated system.' The susceptibility ofa sample sealed in a thin-walled quartz tube was determined to be field independent at room temperature, showing that no ferromagnetic impuritie-s were present. Figure I shows the results of a temperature-dependent study between 30 and 750 K at a magnetic field strength of 14.2 kC. The contribution of the